Crystal Structural Behavior of CoCu₂O₃ at High Temperatures April Jeffries*, Ravhi Kumar, and Andrew Cornelius *Department of Physics, State University of New York at Albany, Albany, NY 12222 University of Nevada, Las Vegas, Las Vegas, NV 89154. Abstract:
Crystal Structural Behavior of CoCu₂O₃ at High TemperaturesApril Jeffries*, Ravhi Kumar, and Andrew Cornelius*Department of Physics, State University of New York atAlbany, Albany, NY 12222University of Nevada, Las Vegas, Las Vegas, NV 89154
High temperature structure of CoCu₂O₃
The spin ladder compounds have received much attention recently due to their relation to the high transition temperature superconductivity. Also the study of spin ladder compounds is of great interest to explore the specific characteristics that result in their behavior. The CoCu₂O₃ spin ladder crystal structure is similar to SrCu₂O₃, which is apparent composition for many high temperature superconductors. The effects of temperature on structural change are investigated for this system. High temperature x-ray diffraction patterns were collected up to 1000⁰C and the variation of lattice parameters as a function of temperature up to decomposition is studied.
The thermal stability of CoCu₂O₃, has been studied at elevated oxygen pressures beyond a high temperature of 1000⁰C . Temperatures at which CoCu₂O₃ undergoes decomposition reactions were studied along with the products of the reactions. The study introduced here provides structural details and the linear coefficient of thermal expansion (CTE) before progressive decomposition.
Powder samples of (Ca1-xCox)Cu₂O₃ (x=0.05) were prepared by the solid state reaction method as described elsewhere . The phase purity of the sample was verified by powder XRD measurements on polycrystalline samples and found to be in single phase. The chemical compositions of the synthesized samples were determined .
High Temperature X-Ray Diffraction:
A circular corundum sample stage was loaded with fine powdered CoCu₂O₃ and loaded into the vacuumed high temperature stage in the Bruker D8 Advance X-Ray Diffractometer (Figure 1). Sample was heated at a rate of 0.5⁰C/sec from 30⁰C to 400⁰C. XRD data was collected at temperatures of 30 ⁰ C, 100 ⁰ C, 200 ⁰ C, 300 ⁰ C, and 400 ⁰ C, then cooled at a rate of 1 ⁰C/sec back to 30 ⁰C for a final collection of data. Another run from 30 ⁰C to 1000 ⁰C was conducted to track the decomposition of the sample. XRD data was collected starting at 30 ⁰C, and every 200 ⁰C up to 1000 ⁰C, and back to 30 ⁰C. TOPAS was used to analyze the x-ray diffraction patterns and the track percent compositions of the sample at various temperatures. Origin8 was used to analyze the data and obtain the linear coefficient of thermal expansion.
• TOPAS was used to display the intensity peaks which are characteristic of the material (Figure 2 and Figure 3) from 30⁰C to 400⁰C. As the temperature increases the shift of the peaks to the lower 2ѳ shows an expansion of the cell.
• Length of lattice parameter vs. temperature data is linear only to 300⁰C, so linear CTE was determined using data from 30⁰C to 300⁰C using Origin8 (Figure 4 a-c).
• Linear CTE for each lattice parameter can be seen in Table 1.
 Buchner, B., et al., Phase diagram features and solidification behaviour of CoCu2O3 at elevated oxygen pressure, Journal of Solid State Chemistry, v. 182, p. 2036, 2009.
 Sekar, C. et al., Synthesis, structural and magnetic properties of spin ladder compound Ca1-xCoxCu2O3, Journal of Magnetism and Magnetic Materials, In Press, Corrected Proof, 2011.
 ASM International. Materials Properties Database Committee, ASM ready reference: Thermal properties of metals, ASM International, p. 560, 2002.
Support from the REU program of the National Science Foundation under grant DMR-1005247 is gratefully acknowledged. The authors thank Dr. Thomas Hartmann and Jerry Egland for assistance with x-ray diffraction equipment and software. Help in data collection and analysis is acknowledged for Daniel Antonio, Patricia Kalita and Jason Baker.
Waterfall plot of XRD data, heating from 30⁰ to 400⁰C, and cooling back to 30⁰.
• In the study by Buchner, at 557⁰C a decomposition of CoCu₂O₃ into CuO and CoO occurs .
The relative percent compositions of the sample between 400⁰C and 600⁰C are shown. The relative percent composition of CuO and CoO increases from 400⁰C to 600⁰C, as the percent composition of CoCu₂O₃ decreases.
•Reactions observed in the previous study  occur at 900⁰C to form CoO and O₂ from Co₃O₄, and at 952⁰C CoCu₂O₃ begins to reform.
Above is the relative percent compositions between 800⁰C and 1000⁰C. The relative percent composition of CoO does not increase and CoCu₂O₃ does not appear to significantly reform from 800⁰C to 1000⁰C.
Zoom of Figure 2 to show a shift to lower angle as temperature increases. A decrease in angle corresponds to an expansion of the cell.
A coefficient of thermal expansion (CTE)is indicative of the amount a structure expands or contracts in response to a temperature change. Linear CTE, α, is determined by the following equation :
α= 1 DL
Where L₀ is the initial length, and DL/DT is the slope of the tangent to the length vs. temperature line. Linear CTE has units of 1/ ⁰C.
• Lattice parameters do not have the same coefficient of thermal expansion, therefore the volume expansion is not isotropic.
• Products of the reaction between 400⁰C and 600⁰C are in good agreement with previous TGA/DTA study .
• CoCu₂O₃ decomposes at 557⁰C . There are no temperature induced phase changes observed before decomposition.
D8 Advance X-Ray Diffractometer